Download presentation

Presentation is loading. Please wait.

Published byAlma Spore Modified about 1 year ago

1
1 University of Waterloo Department of Mechanical Engineering ME Mechanical Design 1 Partial notes – Part 4 (Fatigue) (G. Glinka) Fall 2005

2
2 N i = ? N p = ? N T = ? Metal Fatigue is a process which causes premature irreversible damage or failure of a component subjected to repeated loading. FATIGUE - What is it?

3
3 Metallic Fatigue A sequence of several, very complex phenomena encompassing several disciplines: –motion of dislocations –surface phenomena –fracture mechanics –stress analysis –probability and statistics Begins as an consequence of reversed plastic deformation within a single crystallite but ultimately may cause the destruction of the entire component Influenced by a component’s environment Takes many forms: –fatigue at notches –rolling contact fatigue –fretting fatigue –corrosion fatigue –creep-fatigue Fatigue is not cause of failure per se but leads to the final fracture event.

4
4 The Broad Field of Fracture Mechanics (from Ewalds & Wanhil, ref.3)

5
5 Intrusions and Extrusions: Intrusions and Extrusions: The Early Stages of Fatigue Crack Formation

6
6 Locally, the crack grows in shear; macroscopically it grows in tension. ΔσΔσ ΔσΔσ c Schematic of Fatigue Crack Initiation Subsequent Growth Corresponding and Transition From Mode II to Mode I

7
7 The Process of Fatigue The Process of Fatigue The Materials Science Perspective: Cyclic slip, Cyclic slip, Fatigue crack initiation, Fatigue crack initiation, Stage I fatigue crack growth, Stage I fatigue crack growth, Stage II fatigue crack growth, Stage II fatigue crack growth, Brittle fracture or ductile rupture Brittle fracture or ductile rupture

8
8 Features of the Fatigue Fracture Surface of a Typical Ductile Metal Subjected to Variable Amplitude Cyclic Loading (Collins, ref. 22 ) A – fatigue crack area B – area of the final static failure

9
9 Appearance of Failure Surfaces Caused by Various Modes of Loading Appearance of Failure Surfaces Caused by Various Modes of Loading (SAE Handbook)

10
10 Factors Influencing Fatigue Life Applied Stresses Stress range – The basic cause of plastic deformation and consequently the accumulation of damage Mean stress – Tensile mean and residual stresses aid to the formation and growth of fatigue cracks Stress gradients – Bending is a more favorable loading mode than axial loading because in bending fatigue cracks propagate into the region of lower stresses Materials Tensile and yield strength – Higher strength materials resist plastic deformation and hence have a higher fatigue strength at long lives. Most ductile materials perform better at short lives Quality of material – Metallurgical defects such as inclusions, seams, internal tears, and segregated elements can initiate fatigue cracks Temperature – Temperature usually changes the yield and tensile strength resulting in the change of fatigue resistance (high temperature decreases fatigue resistance) Frequency (rate of straining) – At high frequencies, the metal component may be self-heated.

11
11 Component Geometry Loading History Stress-Strain Analysis Damage Analysis Allowable Load - Fatigue Life Material Properties Information path in strength and fatigue life prediction procedures Strength-Fatigue Analysis Procedure

12
12 Stress Parameters Used in Static Strength and Fatigue Analyses nn y dndn 0 T peak Stress M b) a) nn y dndn 0 T peak Stress S S

13
13 Constant and Variable Amplitude Stress Histories; Constant and Variable Amplitude Stress Histories; Definition of a Stress Cycle & Stress Reversal One cycle mm max min Stress Time 0 Constant amplitude stress history a) Stress Time 0 Variable amplitude stress history One reversal b) In the case of the peak stress history the important parameters are:

14
14 Stress Time Stress history Rainflow counted cycles i-1 i-2 i+1 ii i+2 Stress History and the “Rainflow” Counted Cycles A rainflow counted cycle is identified when any two adjacent reversals in thee stress history satisfy the following relation:

15
15 A rainflow counted cycle is identified when any two adjacent reversals in thee stress history satisfy the following relation : The stress amplitude of such a cycle is: The stress range of such a cycle is: The mean stress of such a cycle is: The Mathematics of the Cycle Rainflow Counting Method for Fatigue Analysis of Stress/Load Histories

16
16

17
17

18
18

19
19

20
20

21
21 Number of Cycles According to the Rainflow Counting Procedure Number of Cycles According to the Rainflow Counting Procedure (N. Dowling, ref. 2)

22
22 The Fatigue S-N method The Fatigue S-N method (Nominal Stress Approach) The principles of the S-N approach (the nominal stress method) Fatigue damage accumulation Significance of geometry (notches) and stress analysis in fatigue evaluations of engineering structures Fatigue life prediction in the design process

23
23 A B Note! In the case of smooth components such as the railway axle the nominal stress and the local peak stress are the same! S min S max Wöhler’s Fatigue Test

24
24 Characteristic parameters of the S - N curve are: S e - fatigue limit corresponding to N = 1 or 2 10 6 cycles for steels and N = 10 8 cycles for aluminum alloys, S fully reversed stress amplitude corresponding to N = 10 3 cycles m - slope of the high cycle regime curve (Part 2) Fully reversed axial S-N curve for AISI 4130 steel. Note the break at the LCF/HCF transition and the endurance limit Number of cycles, N Stress amplitude, S a (ksi) SySy SeSe Part 1Part 2Part 3 Infinite life SuSu S 10 3 Fatigue S-N curve

25
25 Most of available S - N fatigue data has been obtained from fully reversed rotational bending tests. However, material behavior and the resultant S - N curves are different for different types of loading. It concerns in particular the fatigue limit S e. The stress endurance limit, S e, of steels (at 10 6 cycles) and the fatigue strength, S 10 3 corresponding to 10 3 cycles for three types of loading can be approximated as (ref. 1, 23, 24): S 10 3 = 0.90S u and S e = S 10 6 = 0.5 S u - bending S 10 3 = 0.75S u and S e = S 10 6 = S u - axial S 10 3 = 0.72S u and S e = S 10 6 = 0.29 S u - torsion S 10 3 SeSe Number of cycles, Log(N) Relative stress amplitude, S a /S u Torsion Axial Bending

26
26 Approximate endurance limit for various materials: Magnesium alloys (at 10 8 cycles) S e = 0.35Su Copper alloys (at 10 8 cycles) 0.25S u < S e <0.50S u Nickel alloys (at 10 8 cycles) 0.35S u ~~ 48 ksi) Steels (at 10 6 cycles) S e = 0.5S u (if S u ≤ 200 ksi) or S e = 100 ksi (if S u >200 ksi) Irons (at 106 cycles) S e = 0.4S u (if S u ≤ 60 ksi) or S e = 24 ksi (if S u > 60 ksi) S – N curve
~~

27
27 Fatigue Limit – Modifying Factors For many years the emphasis of most fatigue testing was to gain an empirical understanding of the effects of various factors on the base-line S-N curves for ferrous alloys in the intermediate to long life ranges. The variables investigated include: - Rotational bending fatigue limit, S e ’, - Surface conditions, k a, - Size, k b, - Mode of loading, k c, S e = k a k b k c k d k e k f ·S e ’ - Temperature, k d - Reliability factor, k e - Miscellaneous effects (notch), k f Fatigue limit of a machine part, S e

28
28 CaCa Effect of various surface finishes on the fatigue limit of steel. Shown are values of the k a, the ratio of the fatigue limit to that for polished specimens. Below a generalized empirical graph is shown which can be used to estimate the effect of surface finish in comparison with mirror-polished specimens [Shigley (23), Juvinal (24), Bannantine (1) and other textbooks]. Surface Finish Effects on Fatigue Endurance Limit The scratches, pits and machining marks on the surface of a material add stress concentrations to the ones already present due to component geometry. The correction factor for surface finish is sometimes presented on graphs that use a qualitative description of surface finish such as “polished” or “machined”. (from J. Bannantine, ref.1) kaka

29
29 Size Effects on Endurance Limit Fatigue is controlled by the weakest link of the material, with the probability of existence (or density) of a weak link increasing with material volume. The size effect has been correlated with the thin layer of surface material subjected to 95% or more of the maximum surface stress. There are many empirical fits to the size effect data. A fairly conservative one is: The size effect is seen mainly at very long lives. The effect is small in diameters up to 2.0 in (even in bending and torsion). Stress effects in non-circular cross section members In the case of non-circular members the approach is based on so called effective diameter, d e. The effective diameter, d e, for non-circular cross sections is obtained by equating the volume of material stressed at and above 95% of the maximum stress to the same volume in the rotating-bending specimen.

30
max max 0.05d/2 0.95d The material volume subjected to stresses 0.95 max is concentrated in the ring of 0.05d/2 thick. The surface area of such a ring is: The effective diameter, d e, for members with non-circular cross sections * rectangular cross section under bending F 0.95t t Equivalent diameter

31
31 Loading Effects on Endurance Limit The ratio of endurance limits for a material found using axial and rotating bending tests ranges from 0.6 to 0.9. The ratio of endurance limits found using torsion and rotating bending tests ranges from 0.5 to 0.6. A theoretical value obtained from von Mises-Huber- Hencky failure criterion is been used as the most popular estimate.

32
32 From: Shigley and Mischke, Mechanical Engineering Design, 2001 Temperature Effect

33
33 Reliability factor k e The reliability factor accounts for the scatter of reference data such as the rotational bending fatigue limit S e ’. The estimation of the reliability factor is based on the assumption that the scatter can be approximated by the normal statistical probability density distribution. The values of parameter z a associated with various levels of reliability can be found in Table 7-7 in the textbook by Shigley et.al.

34
34 (source: S. Nishijima, ref. 39) S-N curves for assigned probability of failure; P - S - N curves

35
35 Stress concentration factor, K t, and the notch factor effect, k f Fatigue notch factor effect k f depends on the stress concentration factor K t (geometry), scale and material properties and it is expressed in terms of the Fatigue Notch Factor K f.

36
36 1 peak nn 2222 11 33 A D B C F F 2222 2222 2222 3333 3333 C A, B D Stresses in axisymmetric notched body

37
37 Stresses in prismatic notched body A, B, C 2222 2222 2222 3333 D E 11 peak nn 2222 11 33 A DB C F F 1 E

38
38 Stress concentration factors used in fatigue analysis n, S x dndn 0 W peak Stress S nn x dndn 0 W M peak

39
39 Stress concentration factors, K t, in shafts Bending load Axial load S =

40
40 S =

41
41 Similarities and differences between the stress field near the notch and in a smooth specimen x dndn 0 W peak Stress S n =S peak = n =S P

42
42 The Notch Effect in Terms of the Nominal Stress npnp n1n1 S2S2 cycles N0N0 N2N2 S e smooth N ( S) m = C S max Stress range S n2n2 n3n3 n4n4 S Fatigue notch factor!

43
N smooth peak Stress 1 2 N notched M Definition of the fatigue notch factor K f 1 22= peak Stress 2 N notched S SeSe

44
44 PETERSON's approach a – constant, r – notch tip radius; NEUBER’s approach ρ – constant, r – notch tip radius

45
45 The Neuber constant ‘ρ’ for steels and aluminium alloys

46
46 Curves of notch sensitivity index ‘q’ versus notch radius Curves of notch sensitivity index ‘q’ versus notch radius (McGraw Hill Book Co, from ref. 1)

47
47 Plate 1 W 1 = 5.0 in d 1 = 0.5 in. S u = 100 ksi K t = 2.7 q = 0.97 K f1 = 2.65 Illustration of the notch/scale effect Plate 2 W 2 = 0.5 in d 2 = 0.5 i S u = 100 ksi K t = 2.7 q = 0.78 K f1 = 2.32 pea k m1 d1d1 W1W1 pea k d2d2 W2W2 m2

48
48 Procedures for construction of approximate fully reversed S-N curves for smooth and notched components N f (logartmic) Juvinal/Shigley method N f (logartmic) Collins method S ar, ar – nominal/local stress amplitude at zero mean stress m =0 (fully reversed cycle)! f’f’

49
49 Procedures for construction of approximate fully reversed S-N curves for smooth and notched components S ar, ar – nominal/local stress amplitude at zero mean stress m =0 (fully reversed cycle)! S ar (logartmic) N f (logartmic) Manson method 0.9S u ·10 6 S e ’k a k c k b k d k e S e ’k a k c k b k d k e k f SeSe

50
50 NOTE! The empirical relationships concerning the S –N curve data are only estimates! Depending on the acceptable level of uncertainty in the fatigue design, actual test data may be necessary. The most useful concept of the S - N method is the endurance limit, which is used in “infinite-life”, or “safe stress” design philosophy. In general, the S – N approach should not be used to estimate lives below 1000 cycles (N < 1000).

51
51 Constant amplitude cyclic stress histories Fully reversed m = 0, R = -1 Pulsating m = a R = 0 Cyclic m > 0 R > 0

52
52 Mean Stress Effect s m < 0 s m = 0 s m > 0 No. of cycles, logN 2*10 6 Stress amplitude, logS a time s m < 0 s m = 0 s m > 0 Stress amplitude, S a 0

53
53 The tensile mean stress is in general detrimental while the compressive mean stress is beneficial or has negligible effect on the fatigue durability. Because most of the S – N data used in analyses was produced under zero mean stress (R = -1) therefore it is necessary to translate cycles with non- zero mean stress into equivalent cycles with zero mean stress producing the same fatigue life. There are several empirical methods used in practice: The Hiagh diagram was one of the first concepts where the mean stress effect could be accounted for. The procedure is based on a family of S a – S m curves obtained for various fatigue lives. Steel AISI 4340, S y = 147 ksi S y = 147 ksi (Collins)

54
54 Mean Stress Correction for Endurance Limit Gereber (1874) Goodman (1899) Soderberg (1930) Morrow (1960) S a – stress amplitude applied at the mean stress S m ≠ 0 and fatigue life N = 1-2x10 6 cycles. S m - mean stress S e - fatigue limit at S m =0 S u - ultimate strength f ’ - true stress at fracture

55
55 Mean stress correction for arbitrary stress amplitude applied at non-zero mean stress Gereber (1874) Goodman (1899) Soderberg (1930) Morrow (1960) S a – stress amplitude applied at the mean stress S m ≠ 0 and resulting in fatigue life of N cycles. S m - mean stress S ar - fully reversed stress amplitude applied at mean stress S m =0 and resulting in the same fatigue life of N cycles S u - ultimate strength f ’ - true stress at fracture

56
56 Comparison of various methods of accounting for the mean stress effect Most of the experimental data lies between the Goodman and the yield line!

57
57 Approximate Goodman’s diagrams for ductile and brittle materials KfKf KfKf KfKf

58
58 The following generalisations can be made when discussing mean stress effects: 1. The Söderberg method is very conservative and seldom used. 3. Actual test data tend to fall between the Goodman and Gerber curves. 3. For hard steels (i.e., brittle), where the ultimate strength approaches the true fracture stress, the Morrow and Goodman lines are essentially the same. For ductile steels (of > S,,) the Morrow line predicts less sensitivity to mean stress. 4. For most fatigue design situations, R < 1 (i.e., small mean stress in relation to alternating stress), there is little difference in the theories. 5. In the range where the theories show a large difference (i.e., R values approaching 1), there is little experimental data. In this region the yield criterion may set design limits. 6. The mean stress correction methods have been developed mainly for the cases of tensile mean stress. For finite-life calculations the endurance limit in any of the equations can be replaced with a fully reversed alternating stress level corresponding to that finite-life value!

59
59 Procedure for Fatigue Damage Calculation NTNT n 1 n 2 n 3 n 4 cy c le s e N o N 2 e ' N i ( i ) m = a N1N1 N3N3 Stress range,

60
60 n 1 - number of cycles of stress range 1 n 2 - number of cycles of stress range 2 n i - number of cycles of stress range i, - damage induced by one cycle of stress range 1, - damage induced by n 1 cycles of stress range 1, - damage induced by one cycle of stress range 2, - damage induced by n 2 cycles of stress range 2, - damage induced by one cycle of stress range i, - damage induced by n i cycles of stress range i,

61
61 Total Damage Induced by the Stress History It is usually assumed that fatigue failure occurs when the cumulative damage exceeds some critical value such as D =1, i.e. if D > 1 - fatigue failure occurs! For D < 1 we can determine the remaining fatigue life: L R - number of repetitions of the stress history to failure N - total number of cycles to failure

62
62

63
63 Main Steps in the S-N Fatigue Life Estimation Procedure Analysis of external forces acting on the structure and the component in question, Analysis of internal loads in chosen cross section of a component, Selection of individual notched component in the structure, Selection (from ready made family of S-N curves) or construction of S- N curve adequate for given notched element (corrected for all effects), Identification of the stress parameter used for the determination of the S-N curve (nominal/reference stress), Determination of analogous stress parameter for the actual element in the structure, as described above, Identification of appropriate stress history, Extraction of stress cycles (rainflow counting) from the stress history, Calculation of fatigue damage, Fatigue damage summation (Miner- Palmgren hypothesis), Determination of fatigue life in terms of number of stress history repetitions, N blck, (No. of blocks) or the number of cycles to failure, N. The procedure has to be repeated several times if multiple stress concentrations or critical locations are found in a component or structure.

64
64

65
65

66
66

67
67

68
68

69
69

70
70 Results of "rainflow" counting D a m a g e No. SS m S a S a,r (Sm=0) D i =1/N i =1/C*S a -m E E E E E E E E E E E E E E E E n 0 =15 D = E-04 D= D=3.677E-04 L R = 1/D = L R = 1/D = N=n 0 *L R =15* =40680 N=n 0 *L R =15* =40794

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google